|Year : 2015 | Volume
| Issue : 2 | Page : 105-108
|Influence of addition of calcium oxide on physicochemical properties of Portland cement with zirconium or niobium oxide
Mario Tanomaru-Filho1, André Cresto Garcia1, Roberta Bosso-Martelo1, Fabio Luis Camargo V Berbert1, José Mauricio Santos Nunes Reis2, Juliane Maria Guerreiro-Tanomaru1
1 Department of Restorative Dentistry, Araraquara Dental School, São Paulo State University (UNESP), Araraquara, São Paulo, Brazil
2 Department of Prosthodontics, Araraquara Dental School, São Paulo State University (UNESP), Araraquara, São Paulo, Brazil
Click here for correspondence address and email
|Date of Submission||12-Oct-2014|
|Date of Decision||19-Dec-2014|
|Date of Acceptance||23-Dec-2014|
|Date of Web Publication||12-Mar-2015|
| Abstract|| |
Context: Calcium oxide (CaO) may be added to mineral trioxide aggregate (MTA) or Portland cement (PC) to improve physicochemical and biological properties.
Aims: To evaluate the physicochemical properties of PC associated with radiopacifiers and CaO.
Materials and Methods: MTA Angelus, PC + 30% zirconium oxide (Zr), or 30% niobium oxide (Nb) associated with 10 or 20% of CaO were evaluated. Gilmore needles were used to evaluate initial and final setting time. Compressive strength was evaluated after the periods of 24 hours and 21 days. pH was analyzed after 3, 12, 24 hours, 7, 14, 21 days. Solubility and flow tests were performed based on the ISO 6876. The data obtained were submitted to analysis of variance and Tukey tests (P ≤ 0.05).
Results: The associations with 10% CaO showed greater strength that the associations with 20% CaO. The shortest initial setting time was observed for the association PC + Zr + 20% CaO and MTA. All the cements presented alkaline pH. The flow of all cements was similar. The highest solubility was found in the associations with 20% CaO.
Conclusion: The addition of CaO to PC favored the alkaline property and the PC + Zr + 20% CaO presented setting time similar to MTA.
Keywords: Calcium oxide; endodontics; mineral trioxide aggregate; physicochemical properties; portland cement
|How to cite this article:|
Tanomaru-Filho M, Garcia AC, Bosso-Martelo R, Berbert FV, Nunes Reis JS, Guerreiro-Tanomaru JM. Influence of addition of calcium oxide on physicochemical properties of Portland cement with zirconium or niobium oxide. J Conserv Dent 2015;18:105-8
|How to cite this URL:|
Tanomaru-Filho M, Garcia AC, Bosso-Martelo R, Berbert FV, Nunes Reis JS, Guerreiro-Tanomaru JM. Influence of addition of calcium oxide on physicochemical properties of Portland cement with zirconium or niobium oxide. J Conserv Dent [serial online] 2015 [cited 2022 Aug 13];18:105-8. Available from: https://www.jcd.org.in/text.asp?2015/18/2/105/153066
| Introduction|| |
Mineral Trioxide Aggregate (MTA) is a calcium silicate cement indicated to seal communication between pulp cavity and external dental surface.  This material has biocompatibility, antibacterial activity, sealing ability, and bioactivity. , The chemical similarity between MTA and Portland cement (PC) is known, since MTA is composed of PC as its main component.  Bismuth oxide is added to MTA to promote radiopacity. 
MTA has some disadvantages, especially its long setting time, and the presence of bismuth oxide, which alters physicochemical properties.  Zirconium oxide (Zr) promotes adequate radiopacity  and biocompatibility when associated with PC.  Tanomaru-Filho et al., (2012)  observed that the association of PC with Zr has proper physicochemical properties. Niobium oxide (Nb) may also be used as a radiopacifying agent, improving biologic properties of materials. 
In addition to the main components of MTA, such as calcium silicates, CaO may be included in its formulation.  CaO plays an important role in the biological response due its conversion into calcium hydroxide.  Estrela et al., (2012)  and Camilleri et al., (2012)  observed that PC has more CaO in its composition than MTA Angelus. CaO reacts with water and plays an important role in the hydration reaction during setting of the cement. 
The aim of this study was to evaluate the effect of the addition of CaO on the physicochemical and mechanical properties of PC associated with Zr or Nb as radiopacifying agents.
| Materials and methods|| |
The materials evaluated and proportions for manipulation were:
- MTA Angelus (MTA, Angelus, Londrina, Brazil): 1g: 0.3 mL distilled water.
- 60% white PC (PCB-40, Votorantin, Pedro Leopoldo, MG, Brazil) + 30% Zr (Sigma-Aldrich, São Paulo, SP, Brazil) + 10% calcium oxide (Sigma-Aldrich, São Paulo, SP, Brazil) (PC + ZrO 2 + 10% CaO): 1g: 0.27 mL distilled water.
- 60% White PC + 30% Nb (Sigma-Aldrich, São Paulo, SP, Brazil) + 10% CaO (PC + Nb 2 O 5 + 10% CaO): 1g: 0.40 mL distilled water.
- 50% White PC + 30% Zr + 20% CaO (PC + ZrO 2 + 20% CaO): 1g: 0.27 mL distilled water.
- 50% White PC + 30% Nb + 20% CaO (PC + Nb 2 O 5 + 20% CaO): 1g: 0.40 mL distilled water.
The cements were placed in a cylinder mold measuring 6-mm diameter and a thickness of 12 mm, and maintained at 37°C and 95% humidity. After 24 hours and 21 days, they were submitted to compressive test (Emic DL 2000, São José dos Pinhais, PR, Brazil) using a 5KN load cell and 0.5 mm/minute speed. The maximum stress was expressed in MPa.
Setting time test was evaluated in accordance with the ISO 6876 Standard (2002).  Metal rings measuring 10-mm diameter and 1-mm thickness were used (n = 6). The specimens were maintained at 37°C, 95% humidity. For the initial setting time, a Gilmore needle with 100 ±0.5 g and tip diameter of 2 ±0.1 mm was used. For the final setting time, a Gilmore needle with 456 ±0.5 g and tip diameter of 1 ±0.1 mm was used.
For the pH tests, polyethylene tubes measuring 10-mm length and 1-mm diameter were filled with each material (n = 10). Each tube was immersed in 10 mL of distilled water and maintained at 37°C during the experimental periods. At each period, tubes were removed from the flasks and put into new flasks containing 10 mL of distilled water. The experimental time intervals were 3, 12, and 24 hours, 7, 14, and 21 days. The pH of the solutions was measured at each experimental periodo, using a previously calibrated Ultrabasic pH meter (Denver Instrument Company, Arvada, Colorado, USA).
Flow test was evaluated in accordance with ISO 6876 Standard (2002).  After material manipulation, 0.05 mL was placed in the center of a glass plate measuring 4 × 5 cm. Three minutes after manipulation, another glass plate measuring 4 × 5 cm and mass of 20 g was placed. A weight of 100 g was placed on the top, for 7 minutes. Measurements of flow were taken using two methods. In the first technique, largest and smallest diameter of each specimen was measured. Specimens with difference between largest and smallest diameter less than 1 millimeter were used as recommended by the ISO 6876 (2002).  A second evaluation method was used. Specimens were photographed, and the area of cement was measured in mm 2 using a software (UTHSCSA Image Tool for Windows Version 3.00), as described by Tanomaru-Filho et al., (2007),  analyzing gutta-percha flow.
Specimens measuring 1.5 mm thickness and 7.75 mm in internal diameter were fabricated with a nylon thread embedded in the cement mass. The materials were kept at 37°C and 95% humidity, for a period longer than three times the setting time, and placed in a dehumidifier for 7 days. For mass measurement, a precision balance HM-200 (A & D Engineering, Inc., Bradford, MA, USA) was used. The samples were suspended by the nylon thread inside the plastic containers containing 7.5 ml of distilled water. The containers remained in at 37°C for 7 days, when the specimens were removed from the flasks, dried with absorbent paper, and placed in a dehumidifier, until stabilization of mass, when the final mass of each sample was obtained. The solubility value (n = 6) was determined by percentage of mass loss after immersion in water.
The data obtained were submitted to analysis of variance and Tukey test, with significance level set at 5%, using Prism 5.0 (GraphPad Software, San Diego, CA, USA).
| Results|| |
The results showed that MTA has higher compressive strength than other cements. It was observed an increase in the compressive strength for all materials. After 21 days, the associations PC + ZrO 2 + 10% CaO and PC + Nb 2 O 5 + 10% CaO showed greater strength that the associations with 20% CaO, as shown in [Table 1].
|Table 1: Mean values and standard deviation of the compressive strength test after 24 hours and 21 days, the initial and final setting time test, the diameter and area after the flow test, and percentage of loss of mass after the solubility test|
Click here to view
The shortest initial and final setting time was observed for the association PC + ZrO 2 + 20% CaO and MTA (P < 0.05).
All the cements showed alkaline pH [Table 2]. In the three initial periods, 3, 12, and 24 hours, all experimental specimens presented a higher pH value than MTA. In the time periods of 7 and 14 days, all the cements presented a pH similar to MTA. Except association PC + ZrO 2 + 10% CaO, all cements presented a pH higher than MTA after 21 days.
|Table 2: Mean pH values and standard deviation observed for the experimental materials and different periods|
Click here to view
For mean diameter analysis, the lowest value was observed for the association PC + Nb 2 O 5 + 10% CaO, which was similar to the association of PC + Nb 2 O 5 + 20% CaO. In the analysis of area, all cements presented a similar flow (P ≥ 0.05), as observed in [Table 1].
MTA, and PC + 10% CaO with both the radiopacifying agents were statistically similar and presented lower solubility than the association with 20% CaO [Table 1].
| Discussion|| |
CaO plays an important role in biologic response during the mineralization process.  Zr associated with PC resulted in a cement with an adequate radiopacity,  above the minimum value recommended by Specification 57 of ANSI/ADA (ANSI/ADA, 2000).  The association of Zr with PC was shown not to be cytotoxic.  Another chemical element that has been studied for improving the biological properties of materials is Nb, due to its biocompatibility. 
Biomaterials containing CaO have been developed, such as Biodentine. Biodentine is composed of tricalcium silicate, dicalcium silicate, calcium carbonate, CaO, and Zr. 
In this study, the final setting time for MTA (137,8 min) was similar to observed in previous study.  The shortest initial and final setting time was observed for the association PC + ZrO 2 + 20% CaO, which was similar to the MTA initial and final setting time. The shortest setting time of PC + ZrO 2 when CaO was added, may be related to the hydration of the cement in the presence of CaO, which leads to calcium hydroxide formation, as demonstrated by Camilleri et al., (2013).  A longer setting time was observed when Nb was used as radiopacifying agent, which may be related to the larger quantity of water used for material manipulation.  Tanomaru-Filho et al., (2012)  observed that the addition of ZrO 2 to white PC presented an initial setting time similar to MTA, and reduction of the final setting time in comparison to pure PC.
An increase in the compressive strength was observed for all materials. The incorporation of additives to MTA has been shown to decrease its strength.  In the present study, MTA showed a higher compressive strength than other MTA associations, which may be explained by the larger quantity of CaO in the cements. , Camilleri et al., (2013)  observed that CaO has large particle size and this component may not reacts during the hydration process.
The obtained results in the present study showed that cements associated with 20% CaO have higher solubility. Húngaro Duarte et al., (2012)  demonstrated that white MTA presents a higher solubility than white PC or the association PC with ZrO 2 . The cements MTA and PC + 10% CaO associated with ZrO 2 and Nb 2 O 5 presented lower solubility than the association with 20% CaO. The results in the present study showed that the MTA and PC + 10% CaO cements associated with ZrO 2 or Nb 2 O 5 are in accordance with ANSI/ADA No. 57 (2008),  which established that the solubility must be lower than 3%.
All the cements presented an alkaline pH. Analyses in the periods of 3, 12, 24 hours, and 21 days, showed that experimental cements presented a higher pH than MTA, except the association PC + ZrO 2 + 10% CaO after 21 days, which was similar to MTA. This alkalinity is a result of the calcium hydroxide produced during hydration. Calcium hydroxide releases calcium and hydroxyl ions.
The flow of retrofilling materials may favor retrograde filling and sealing. Using area analysis, all cements presented similar flow. In the analysis of mean diameter, a greater flow was observed for the associations with 20% CaO, and the association of 10% CaO and ZrO 2 . The flow observed for MTA Angelus was in agreement with Camilleri (2009)  for white Pro Root MTA.
It was concluded that the addition of CaO to PC favored the alkaline propertyl and the association PC + ZrO 2 + CaO presented potential for clinical use. Additional studies on the biocompatibility and bioactivity of the material must be conducted.
| Acknowledgements|| |
This study received financial support from PIBIC/Cnpq.
| References|| |
Lee SJ, Monsef M, Torabinejad M. Sealing ability of a mineral trioxide aggregate for repair of lateral root perforations. J Endod 1993;19:541-4.
Parirokh M, Torabinejad M. Mineral trioxide aggregate: A comprehensive literature review - Part III: Clinical applications, drawbacks, and mechanism of action. J Endod 2010;36:400-13.
Malik G, Bogra P, Singh S, Samra RK. Comparative evaluation of intracanal sealing ability of mineral trioxide aggregate and glass ionomer cement: An in vitro
study. J Conserv Dent 2013;16:540-5.
Camilleri C. The chemical composition of mineral trioxide aggregate. J Conserv Dent 2008;11:141-3.
Asgary S, Eghbal MJ, Parirokh M, Ghoddusi J, Kheirieh S, Brink F. Comparison of mineral trioxide aggregate's composition with Portland cements and a new endodontic cement. J Endod 2009;35:243-50.
Coomaraswamy KS, Lumley PJ, Hofmann MP. Effect of bismuth oxide radiopacifier content on the material properties of an endodontic Portland cement-based (MTA-like) system. J Endod 2007;33:295-8.
Húngaro Duarte MA, de Oliveira El Kadre GD, Vivan RR, Guerreiro Tanomaru JM, Tanomaru Filho M, de Moraes IG. Radiopacity of Portland cement associated with different radiopacifying agents. J Endod 2009;35:737-40.
Gomes Cornélio AL, Salles LP, Campos da Paz M, Cirelli JA, Guerreiro-Tanomaru JM, Tanomaru Filho M. Cytotoxicity of Portland cement with different radiopacifying agents: A cell death study. J Endod 2011;37:203-10.
Tanomaru-Filho M, Morales V, da Silva GF, Bosso R, Reis JM, Duarte MA, et al
. Compressive strength and setting time of MTA and Portland cement associated with different radiopacifying agents. ISRN Dent 2012;2012:898051.
Denry IL, Holloway JA, Nakkula RJ, Walters JD. Effect of niobium content on the microstructure and thermal properties of fluorapatite glass-ceramics. J Biomed Mater Res B Appl Biomater 2005;75:18-24.
Camilleri J, Sorrentino F, Damidot D. Investigation of the hydration and bioactivity of radiopacified tricalcium silicate cement, Biodentine and MTA Angelus. Dent Mater 2013;29:580-93.
Estrela C, Sousa-Neto MD, Guedes OA, Alencar AH, Duarte MA, Pécora JD. Characterization of calcium oxide in root perforation sealer materials. Braz Dent J 2012;23:539-46.
Camilleri J, Kralj P, Veber M, Sinagra E. Characterization and analyses of acid-extractable and leached trace elements in dental cements. Int Endod J 2012;45:737-43.
Crisp S, Wilson AD. Reactions in glass ionomer cements: V. Effect of incorporating tartaric acid in the cement liquid. J Dent Res 1978;55:1023-31.
International Standards Organization. Dental root canal sealing materials. ISO 6876; 2002. p. 7-8.
Tanomaru-Filho M, Silveira GF, Tanomaru JM, Bier CA. Evaluation of the thermoplasticity of different gutta-percha cones and Resilon. Aust Endod J 2007;33:23-6.
ANSI/ADA. Specification No. 57: Endodontic sealing materials. Chicago, IL: ANSI/ADA; 2000.
Gandolfi MG, Iacono F, Agee K, Siboni F, Tay F, Pashley DH, et al
. Setting time and expansion in different soaking media of experimental accelerated calcium-silicate cements and ProRoot MTA. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2009;108:39-45.
Stefanou GD, Larsinos CH. Influence of mixing water on the setting time of concrete. Int J Cement Compos Lightweight Concrete 1981;3:45-8.
Kogan P, He J, Glickman GN, Watanabe I. The effects of various additives on setting properties of MTA. J Endod 2006;32:569-72.
Húngaro Duarte MA, Minotti PG, Rodrigues CT, Zapata RO, Bramante CM, Tanomaru Filho M, et al
. Effect of different radiopacifying agents on the physicochemical properties of white Portland cement and white mineral trioxide aggregate. J Endod 2012;38:394-7.
Camilleri J. Evaluation of selected properties of mineral trioxide aggregate sealer cement. J Endod 2009;35:1412-7.
Rua Humaitá, 1680, Caixa Postal 331, Centro - 14801-903, Araraquara, São Paulo
Source of Support: None, Conflict of Interest: None
[Table 1], [Table 2]
|This article has been cited by|
Effect of the addition of nanoparticles of
and different water-to-powder ratios on the physicochemical properties of white Portland cement
| ||Cleonice da Silveira Teixeira, Jessica Coelho Wasielewsky, Giovanna Slongo Santos, Anarela Bernardi, Eduardo Antunes Bortoluzzi, Lucas da Fonseca Roberti Garcia |
| ||Microscopy Research and Technique. 2021; 84(4): 592 |
|[Pubmed] | [DOI]|
||Concentrated MTA Repair HP reduced biofilm and can cause reparative action at a distance
| ||Poliana Amanda Oliveira Silva, Stella Maris de Freitas Lima, Danilo César Mota Martins, Ingrid Aquino Amorim, Cristiano Lacorte, Jeesser Alves Almeida, Octávio Luiz Franco, Taia Maria Berto Rezende |
| ||International Endodontic Journal. 2021; 54(10): 1925 |
|[Pubmed] | [DOI]|
||Chemical modification of MTA and CEM cement to decrease setting time and improve bioactivity properties by adding alkaline salts
| ||Faeze Jamali Zavare, Hanieh Nojehdehian, Maryam Moezizadeh, Mehdi Daneshpooya |
| ||Journal of Dental Research, Dental Clinics, Dental Prospects. 2020; 14(1): 1 |
|[Pubmed] | [DOI]|
||Addition of a Fluoride-containing Radiopacifier Improves Micromechanical and Biological Characteristics of Modified Calcium Silicate Cements
| ||Djordje Antonijevic, Anke Jeschke, Bozana Colovic, Petar Milovanovic, Danimir Jevremovic, Danilo Kisic, Annika vom Scheidt, Michael Hahn, Michael Amling, Vukoman Jokanovic, Björn Busse, Marija Djuric |
| ||Journal of Endodontics. 2015; 41(12): 2050 |
|[Pubmed] | [DOI]|